Rational (supra)molecular design and catalytic activity of cage-like Cu<sub>4</sub>-based phenylsilsesquioxanes.
Zueva, Anna Y.; Bilyachenko, Alexey N.; Khrustalev, Victor N.; Shul'pina, Lidia S.; Ikonnikov, Nikolay S.; Dorovatovskii, Pavel V.; Shubina, Elena S.; Ragimov, Karim; Lobanov, Nikolai N.; Sun, Di; Nanoscale 16 (2024) 18389–18398; doi:10.1039/d4nr02173h

data_1572462
_publ_section_title
;
 Rational (supra)molecular design and catalytic activity of cage-like
 Cu<sub>4</sub>-based phenylsilsesquioxanes.
;
_journal_issue                   39
_journal_name_full               Nanoscale
_journal_page_first              18389
_journal_page_last               18398
_journal_paper_doi               10.1039/d4nr02173h
_journal_volume                  16
_journal_year                    2024
_chemical_formula_moiety         'C92 H112 Cu4 Na4 O30 Si12'
_chemical_formula_sum            'C92 H112 Cu4 Na4 O30 Si12'
_chemical_formula_weight         2381.06
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     difmap
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2013
_audit_update_record
;
2024-05-14 deposited with the CCDC.	2024-08-22 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 136.955(5)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   42.5782(11)
_cell_length_b                   12.84264(11)
_cell_length_c                   28.6065(7)
_cell_measurement_reflns_used    37983
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      76.591
_cell_measurement_theta_min      3.016
_cell_volume                     10677.1(11)
_computing_cell_refinement       'CrysAlisPro 1.171.41.117a (Rigaku OD, 2021)'
_computing_data_collection       'CrysAlisPro 1.171.41.117a (Rigaku OD, 2021)'
_computing_data_reduction        'CrysAlisPro 1.171.41.117a (Rigaku OD, 2021)'
_computing_molecular_graphics    'SHELXTL (Sheldrick, 2015)'
_computing_publication_material  'SHELXTL (Sheldrick, 2015)'
_computing_structure_refinement  'SHELXL (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measurement_device_type  'XtaLAB Synergy, Dualflex, HyPix'
_diffrn_measurement_method       '\f and \w'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0636
_diffrn_reflns_av_unetI/netI     0.0286
_diffrn_reflns_Laue_measured_fraction_full 0.995
_diffrn_reflns_Laue_measured_fraction_max 0.987
_diffrn_reflns_limit_h_max       53
_diffrn_reflns_limit_h_min       -53
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       36
_diffrn_reflns_limit_l_min       -36
_diffrn_reflns_number            130953
_diffrn_reflns_point_group_measured_fraction_full 0.995
_diffrn_reflns_point_group_measured_fraction_max 0.987
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         78.016
_diffrn_reflns_theta_min         3.041
_diffrn_source                   'micro-focus sealed X-ray tube'
_exptl_absorpt_coefficient_mu    2.980
_exptl_absorpt_correction_T_max  0.900
_exptl_absorpt_correction_T_min  0.529
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.42.79a (Rigaku Oxford Diffraction, 2022)
Numerical absorption correction based on gaussian integration over
a multifaceted crystal model
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    1.481
_exptl_crystal_description       'prismatic needle'
_exptl_crystal_F_000             4928
_exptl_crystal_size_max          0.23
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.02
_refine_diff_density_max         2.033
_refine_diff_density_min         -1.169
_refine_diff_density_rms         0.120
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.072
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     436
_refine_ls_number_reflns         11284
_refine_ls_number_restraints     137
_refine_ls_restrained_S_all      1.078
_refine_ls_R_factor_all          0.0908
_refine_ls_R_factor_gt           0.0819
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.09P)^2^+90P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2056
_refine_ls_wR_factor_ref         0.2125
_reflns_Friedel_coverage         0.000
_reflns_number_gt                9658
_reflns_number_total             11284
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d4nr02173h2.cif
_cod_data_source_block           6a
_cod_depositor_comments
'Adding full bibliography for 1572445--1572463.cif.'
_cod_original_cell_volume        10677.2(11)
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               1572462
_shelx_estimated_absorpt_t_min   0.547
_shelx_estimated_absorpt_t_max   0.943
_shelxl_version_number           2013-4
_shelx_res_checksum              91159